# Accurate Theory for Thermal Elastic-Plastic Analysis to ... 40 Accurate Theory for Thermal...

date post

04-Jun-2018Category

## Documents

view

212download

0

Embed Size (px)

### Transcript of Accurate Theory for Thermal Elastic-Plastic Analysis to ... 40 Accurate Theory for Thermal...

39

Transactions of JWRI, Vol.43 (2014), No. 1

Accurate Theory for Thermal Elastic-Plastic Analysis

to Significantly Shorten Computation Time

NAKACHO Keiji*

Abstract

The thermal elastic-plastic analysis of the transient and residual stresses and the deformations that occur during welding requires a long computation time to obtain accurate results. The reason for this is the necessity for the temperature increment to be sufficiently small to ensure calculation accuracy. In this study, the thermal elastic and thermal elastic-plastic constitutive equations were modified to enable the use of very large temperature increments. Moreover, in the latter constitutive equation, the definition of the differential coefficient of the yield stress when the temperature changes is ingeniously modified to perfectly satisfy the yield condition. The new constitutive equations were introduced into the FEM (Finite Element Method) program. A simple typical problem of thermal elastic-plastic mechanics was analyzed to verify the basic capability of the new theory. Further, to examine the reliability and accuracy of the theory, a complex welding problem was analyzed. The computed welding residual stress and deformation were compared with the accurate results obtained by the usual incremental method using very small temperature increments, and those obtained by ABAQUS. High accuracy was confirmed, and the computation was found to be significantly shortened (reduced by one order) compared to those of the usual incremental method and ABAQUS.

KEY WORDS: (thermal elastic-plastic analysis), (shortening of computation time), (refined constitutive equation), (finite element method), (welding stress and deformation)

1. Introduction The thermal elastic-plastic analysis of the transient and residual stresses and the deformations that occur during welding is done using the incremental method [13] because of the non-linear behavior and the dependency on the temperature history. The temperature increment used for the analysis has to be sufficiently small to ensure calculation accuracy. The analysis [411] therefore requires long computation time. In this study, the thermal elastic and thermal elastic-plastic constitutive equations are modified to enable the use of very large temperature increments. Moreover, in the latter constitutive equation, the definition of the differential coefficient of the yield stress when the temperature changes is ingeniously modified to perfectly satisfy the yield condition. The new constitutive equations are effective, simple, and can be easily introduced into the usual FEM (Finite Element Method) program for thermal elastic-plastic analysis. A simple typical problem of thermal elastic-plastic mechanics was analyzed to verify the basic capability of the new theory. To examine the reliability and accuracy of the theory, a complex welding problem was also

analyzed. The results (the welding residual stress and deformation) were compared with the accurate results obtained by the usual incremental method using a very small temperature increment, and those obtained by ABAQUS. 2. New Accurate Incremental Theory of Thermal Elastic-Plastic Analysis for Large Temperature Increment The new accurate thermal elastic and thermal elastic-plastic constitutive equations are developed here, and can be used for very large temperature increments. 2.1 Difficulties of Using Large Temperature Increment The two major reasons why it is difficult to increase the temperature increment during thermal elastic-plastic analyses, especially those of the mechanical phenomena of welding, are as follows: (a) The material properties change with respect to the temperature and its history. Especially in welding, the temperature range is very wide. The changes in the material properties are therefore significant.

Received on June 30, 2014 * Associate Professor

Transactions of JWRI is published by Joining and Welding Research Institute, Osaka University, Ibaraki, Osaka 567-0047, Japan

40

Accurate Theory for Thermal Elastic-Plastic Analysis to Significantly Shorten Computation Time

(b) When the stress becomes large, the stress state may change from elastic to plastic. In the incremental method, the change occurs incrementally. If the calculation is performed for the elastic state, the equivalent stress after the increment may significantly exceed the yield stress; that is, the stress point may largely fly across the yield surface in the stress space. To use large temperature increments and maintain high accuracy, these behaviors should be sufficiently considered and managed in the theory. Regarding problem (a) above, it is necessary to take into account the temperature and its history and how they affect the material properties, regardless of the magnitude of the temperature increment. Moreover, for large temperature increments, the temperature, which determines the material property, becomes more important for accurate analysis. Regarding problem (b) above, the error that results from going beyond the yield surface is an important issue, especially when large temperature increments are used. The error may increase as the increment increases. Accordingly, if a large temperature increment is used, the theory should include a function that prevents the stress point from exceeding the yield surface during the increment, or a modification function that returns the stress point to the yield surface during the next increment. In this paper, a new theory that includes the latter function will be proposed. The denotations of the superscripts and subscripts used in equations in subsequent sections are as follows: a : initial value in the increment c : final value in the increment a c : mean value during the increment ac : coefficient intermingled of initial, final, and mean values c a : incremental value 2.2 Accurate Elastic Constitutive Equation for Large Temperature Increment A very accurate constitutive equation is derived for the case in which the elastic state is maintained during large temperature increments. (a) Thermal strain increment

dT

ca

dT

ca

= { }ac dTca (1)

where { }ac

is the instantaneous linear expansion

coefficient, and dTca is the temperature increment. (b) Total strain increment

d{ }ca

d{ }ca = de

ca

+ dT

ca

(2)

where

de

ca

is the elastic strain increment.

(c) Stress-elastic strain relationship

{ } = De(T )

e

(3)

where { } is the stress, e

is the elastic strain, and

De(T )

is the elastic matrix (composed of the Youngs

modulus and the Poissons ratio, which are temperature-dependent, and (T) is omitted below). The most important relationship that must be satisfied at all times in the elastic state and the elastic-plastic state is that between the stress and the elastic strain; that is, Eq. (3). Like Eq. (4), Eq. (3) must be satisfied for all temperatures during the increment.

{ }a = D

e

a

e

a

{ }c = D

e

c

e

c

(4)

{ }c = { }a + d{ }ca

De c

e

c

= De a

+ d De ca

e

a

+ de

ca

where

d{ }ca is the stress increment, and

d De ca

= d De c d De

a

=De

c De

a

dTca

dTca =d De

dT

ac

d Tca

(5) The relationship between the stress increment and the elastic strain increment is obtained from Eq. (4).

d{ }ca = D

e

c

d e

ca

+ d De ca

e

a

(6)

(d) Incremental stress-total strain relationship (the elastic constitutive equation) The incremental constitutive equation for the elastic state is derived from Eqs. (1), (2), and (6). Equation (7) is the accurate elastic constitutive equation, which sufficiently considers the temperatures required to determine the material properties. Using Eq. (7), Eq. (3) is satisfied after the increment, even if the temperature increment is very large.

d{ }ca = D

e

c

d{ }ca Ce

ac

dTca (7)

where

Ce

ac

= De c

{ }ac De

c

1 d De

dT

ac

e

a

2.3 Accurate Elastic-Plastic Constitutive Equation for Large Temperature Increment A very accurate constitutive equation is derived for the case in which the elastic-plastic state is maintained during a large temperature increment.

41

Transactions of JWRI, Vol.43 (2014), No. 1

(a) Total strain increment

d{ }ca

d{ }ca = d

e

ca

+ d p

ca

+ dT

ca

(8)

where

d p

ca

is the plastic strain increment.

(b) Yield function (strain-hardening rule)

f (ij ij ,o )

In this theory, the incremental strain theory (the flow theory) is assumed, and the combined strain-hardening rule is applied to the yield function, in which the yield surface can change both the size and the position. The size of the yield surface depends on the total plastic strain and the temperature. The yield surface (yield condition) and the change of in size are related by f (ij ij ,o ) = 0 (9)

where { } is the center of the yield surface, o is the

size of the yield surface, o =o(p, T ) , and

p is the

magnitude of the total

*View more*